New insights into the structural properties of κ-(BEDT-TTF)~2~Ag~2~(CN)~3~ spin liquid
Foury-Leylekian, Pascale; Ilakovac, Vita; Fertey, Pierre; Baledent, Victor; Milat, Ognjen; Miyagawa, Kazuya; Kanoda, Kazushi; Hiramatsu, Takaaki; Yoshida, Yukihiro; Saito, Gunzi; Alemany, Pere; Canadell, Enric; Tomic, Silvia; Pouget, Jean-Paul; Acta Crystallographica Section B 76 (2020) –; doi:10.1107/S2052520620005545

data_2108624
_publ_section_title
;
 New insights into the structural properties of
 \k-(BEDT-TTF)~2~Ag~2~(CN)~3~ spin liquid
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first
;
;
_journal_paper_doi               10.1107/S2052520620005545
_journal_volume                  76
_journal_year                    2020
_chemical_formula_moiety         'C3 Ag2 N3, 2(C10 H8 S8)'
_chemical_formula_sum            'C23 H16 Ag2 N3 S16'
_chemical_formula_weight         1063.17
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                90.012(2)
_cell_angle_beta                 91.364(2)
_cell_angle_gamma                89.9980(10)
_cell_formula_units_Z            2
_cell_length_a                   15.0831(3)
_cell_length_b                   8.64470(10)
_cell_length_c                   13.4755(3)
_cell_measurement_reflns_used    26905
_cell_measurement_temperature    293
_cell_measurement_theta_max      32.04
_cell_measurement_theta_min      2.55
_cell_volume                     1756.56(6)
_computing_cell_refinement       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_diffrn_ambient_temperature      293
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.2930
_diffrn_measured_fraction_theta_full 0.9555
_diffrn_measured_fraction_theta_max 0.78
_diffrn_measurement_device_type  'Xcalibur, Atlas'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_monochromator  synchrotron
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.6717
_diffrn_reflns_av_R_equivalents  0.0485
_diffrn_reflns_av_unetI/netI     0.0793
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            11624
_diffrn_reflns_reduction_process 'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_diffrn_reflns_theta_full        24.83
_diffrn_reflns_theta_max         32.39
_diffrn_reflns_theta_min         1.89
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    1.746
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.893
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.46 (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_density_diffrn    2.0554
_exptl_crystal_description       plate
_exptl_crystal_F_000             1050
_refine_diff_density_max         1.18
_refine_diff_density_min         -1.00
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    2.67
_refine_ls_goodness_of_fit_ref   2.41
_refine_ls_hydrogen_treatment    constr
_refine_ls_number_constraints    16
_refine_ls_number_parameters     397
_refine_ls_number_reflns         11624
_refine_ls_number_restraints     2
_refine_ls_R_factor_all          0.0577
_refine_ls_R_factor_gt           0.0470
_refine_ls_shift/su_max          0.0188
_refine_ls_shift/su_mean         0.0014
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0656
_refine_ls_wR_factor_ref         0.0672
_reflns_number_gt                9553
_reflns_number_total             11624
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            lo5067sup1.cif
_cod_data_source_block           300K
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_diffrn_radiation_probe' value 'X-ray' was changed to
'x-ray' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/IUCr/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_original_formula_sum        'C23 H16 S16 N3 Ag2'
_cod_database_code               2108624
_cod_database_fobs_code 2108624